Anuncio

INVESTIGACIÓN REVISTA MEXICANA DE FÍSICA 50 (6) 614–619 DICIEMBRE 2004 Subband structure comparison between n- and p-type double delta-doped GaAs quantum wells I. Rodriguez-Vargas and L.M. Gaggero-Sager Facultad de Ciencias, Universidad Autónoma del Estado de Morelos, Av. Universidad 1001, Col. Chamilpa 62210 Cuernavaca, Morelos, México Recibido el 26 de marzo de 2004; aceptado el 18 de agosto de 2004 We compute the electron level structure (n-type) and the hole subband structure (p-type) of double δ-doped GaAs (DDD) quantum wells, considering exchange effects. The Thomas-Fermi (TF), and Thomas-Fermi-Dirac (TFD) approximations have been applied in order to describe the bending of the conduction and valence band, respectively. The electron and the hole subband structure study indicates that exchange effects are more important in p-type DDD quantum wells than in n-type DDD. Also our results agree with the experimental data available. Keywords: δ-doped quantum wells; electron and hole states; exchange effects. Calculamos la estructura de niveles electrónicos (tipo-n), ası́ como la de huecos (tipo-p) de pozos cuánticos δ-dopados dobles (DDD) en GaAs. Se han tomando en cuenta los efectos de intercambio en el estudio. Las aproximaciónes de Thomas-Fermi (TF) y Thomas-FermiDirac (TFD) han sido implementadas para describir el doblamiento de la banda de conducción y de valencia respectivamente. El estudio de la estructura de niveles electrónicos y de huecos revela que los efectos de muchos cuerpos son más importantes en los pozos DDD tipo-p que en los DDD tipo-n. De la misma manera nuestros resultados están en buen acuerdo con los datos experimentales disponibles. Descriptores: Pozos δ-dopados; estructura electrónica; efectos de muchos cuerpos. PACS: 73.30; 73.61; S5.11 1. Introduction Nowadays, control and precision in growth and doping techniques allow the fabrication of systems where the impurity deposition is made with atomic resolution. A two dimensional electron (2DEG) or hole gas (2DHG) is formed if the impurity doping is made in an atomic plane (δ-doping technique), in such a way that the impurity density be enough to the effective Bohr radii between donors (n-type) or acceptors (p-type) overlapped. The foremention situation was firstly proposed by Wood [1], and later brought it about by Ploog [2]; calling it a δ-doped quantum well n- or p-type, depending on whether we are working with donors or acceptors. The δ-doping technique is a useful tool in the fabrication of high power devices, and also for its possible technological applications in δ-FET [6,7], and ALD-FET [8] (where a δ-doped quantum well is used as a channel between the terminals of the transistor). There are several works in n- [3-8] and p-type [9-15] single δ-doped quantum wells (SDD). Thomas-Fermi (TF) and Thomas-Fermi-Dirac (TFD) approximations have demonstrated to be useful tools in the theoretical treatment of δ-doped quantum wells [16-18]. The main advantage of these approximations is the possibility of obtaining an analytical solution to the Poisson equation. This allows us to avoid a long and troublesome self-consistent (SC) calculation. When the exchange effects are taken into account explicitly in the TF energy density functional, we are concerned with the TFD theory, i.e., the generalization of the TF approximation. It is important to mention that the TFD theory is not applicable to describe the conduction band bending because the electron density n(r) does not tend to zero at infinity, a physical requirement in δ-doped quantum wells. The situation drastically changes when the carriers, responsible of the conduction, are holes, because the effective masses are negative and this avoids the algebraic origin of the above mentioned problems. As a consequence, the solution in this case is SC and satisfactory [18]. On the other hand, from the theoretical point of view, only a few works in DDD quantum wells are reported in Refs. 19 to 21. DDD quantum wells are very interesting as far as the device industry is concerned, since by the interlayer distance between wells and the impurity density varies, an improvement in the transport properties is achieved [22-24]. The present paper is devoted to the subband structure study in both n- and p-type DDD quantum wells. TF and TFD approximations are implemented in order to accomplish the level structure calculation. The many-body effects are also included to discern their relevance in the electron and hole level structure. A comparison between both systems is given, in the same way that our results are confronted versus the experimental data available. Next section includes mathematical models followed with results, and finally with conclusions. 2. 2.1. Mathematical Models TF theory applied to n-type DDD GaAs quantum wells Consider a GaAs matrix doped at atomic precision with a donor density n2D of Si atoms in two of its planes, located at a certain distance l (the same impurity density is assumed SUBBAND STRUCTURE COMPARISON BETWEEN N - AND P -TYPE DOUBLE DELTA-DOPED GAAS QUANTUM WELLS in both planes). The effective potential created by the 2DEG, and the ionized impurities causes a conduction band bending. We have used the TF theory in order to obtain an analytical solution for this potential [20]. VH − µ = − α2 , (α |z + l/2| + z0n )4 (1) where α = 2/15π, and z0n = (α3 /πn2D )1/5 . But our survey is engaged in the study of exchange effects. The inclusion of the many-body effects is made through the Local Density Approximation (LDA), thereby the exchange potential is: 2 (2) Vx (z) = − (3π 2 (a∗0 )3 n(z))1/3 Ry∗ , π where a∗0 = r 2 /(e2 m∗ ), and Ry∗ = e2 /(2r a∗0 ) are the effective Bohr radius, and the effective Rydberg constant. The rest of the equations presented in this subsection will be in effective units. The exchange potential can be written in terms of the Hartree potential, due to the relation between n(z) and VH (z) [20] 2 (3) Vx (z) = − (µ − VH (z))1/2 . π Finally substituting (1) in (3) the total potential V = VH + Vx is 2 α2 α − . (4) V (z)=− (α |z + l/2| +z0n )4 π (α |z + l/2| +z0n )2 2.2. TFD theory in p-type DDD GaAs quantum wells Again, a GaAs matrix has been considered, but instead of donor impurities, acceptor impurities are used to dope the system. Two planes of the host material are δ-doped (located at a distance l), with an impurity density p2D . The acceptor impurities cause the presence of a 2DHG. Both ionized impurities, and 2DHG are responsible for the valence band bending, that in this case, we will describe it in terms of the TFD approximation. First of all, it is important to take notice of the hole ladders: the heavy (hh), the light (lh), and the split-off (so) holes. In our study, only hh and lh bands are taken into account, since the potential depth never exceeds the energy distance to the so band for the range of impurity density considered here (p2D ≤ 1 × 1013 cm−2 ). This is shown in p-type SDD GaAs quantum wells [17]. The kinetic energy-density functional, the density functional associated to the interaction between 2DHG, the impurity planes, as well as the density functional concerning to the hole-hole interaction come as in Ref. 20. The exchangeenergy functional is given by Ref. 18, adding the aforementioned terms we have ET F D , 2/3 e2 π 3 p(z) 3π 2 3 p(z) dz − , ET F D = 10med r 3a∗ p(z )p(z) |z − z | dzdz − ς(w) 0 (3π 2 )1/3 Ry∗ , 2π 2πe2 p(z)4/3 dz + p2D p(z){|z + l/2| + |z − l/2|}, (5) r 615 where p(z) is the hole density, p2D is the bi-dimensional impurity concentration, 2/3 med = mhh 1 + (mlh /mhh )3/2 = mhh ma , w = mlh /mhh , a∗0 = r 2 /e2 mhh , Ry∗ = e2 /2r a∗0 , and ς(w) = 2−1/3 + (1 − w2 )[w2 (aw + b) + c(4w3 + 3w2 + 2w + 1)] [18]. Using the variational principle δ(ET F D − µN ) = 0, with N= p(z)dz, we obtain µ∗ = 3π 2 pau (z) 2/3 3/2 ma 2 (z), + VH∗ − ς(w) p1/3 π au (6) where pau (z) = (a∗0 )3 p(z), VH∗ = VH /Ry∗ , and µ∗ = µ/Ry∗ . 1/3 Therefore resolving the quadratic equation for pau , and taking into account the physically meaningful solution, 3 π 2 (µ∗ − VH∗ (z)) m3a ς 3 (w) 1− 1+ . (7) pau (z) = 3π 5 ς 2 (w)ma The exchange potential is 2 Vx∗ (z) = −ς(w) (3π 2 )1/3 p1/3 au (z), π (8) and using the direct relation between pau (z) and VH∗ , we find Vx∗ (z)= π 2 (µ∗ −VH∗ (z)) 2ς 2 (w)ma 1− 1+ . − π2 ς 2 (w)ma (9) We can restrict to z ≤ 0, since the potential is an even function as in the case of n-type DDD quantum wells: π 2 (µ∗ − VH∗ ) dVH∗ (z) 8m3a ς 3 (w) 1− 1+ =− dz 2 3π 4 ma ς 2 (w) +8πp2D δ(z + l/2). (10) At this point, it is important to stress that in order to take advantage of the present model, we discard modifications in the form of the Hartree potential due to the exchange effects, while in the level structure and the charge density, these changes are available. Under these conditions the solution for Rev. Mex. Fı́s. 50 (6) (2004) 614–619 616 I. RODRIGUEZ-VARGAS AND L.M. GAGGERO-SAGER TABLE I. Paramount features of n-type DDD GaAs quantum wells in the low, intermediate, and high density limit: degeneracy distance ldeg , quantum well depth V0 and degeneracy-energy difference between excited electron states and the basic level ∆E01 = E0 − E1 , ∆E02 = E0 − E2 , etc., the superscripts o and x denote omitting and considering exchange effects respectively ( the energy is in meV, the distance in Å and the impurity density in units of 1012 cm−2 ). n2D o ldeg E0 E1 1 400 700 4 250 400 10 160 250 x ldeg o ∆E01 x ∆E01 −18.9 −22.3 o ∆E02 x ∆E02 V0o V0x −50.7 −61.7 E0 E1 360 640 570 230 280 530 −57.1 −61.6 −75.9 −83.4 −153.9 −172.9 380 160 240 360 −113.1 −118.7 −155.8 −165.3 −318.9 −346.4 E2 E2 VH∗ is of the form 1/f 4 (z), where f (z) is a linear function of z [20], VH∗ − µ∗ = − β2 , (β |z + l/2| + z0p )4 (11) 3/2 with β = 2ma /15π, and z0p = (β 3 /πp2D )1/5 . Hence the total potential V ∗ = VH∗ + Vx∗ is difference that the width of the SDD quantum well increases as interlayer distance of the DDD does. Therefore the wave functions look like the wave functions of a SDD quantum well (Fig. 3). • The drop of the electron levels halts at a certain distance, depending on the energy level considered, and then the DDD characteristic onset surmounts the SDD ones, as a consequence, the energy levels go up. β2 2ς 2 (w)ma − (β |z + l/2| + z0p )4 π2 β2 π2 (12) × 1− 1+ 2 ς (w)ma (β |z + l/2| + z0p )4 V∗ =− The last equation allows us to avoid a long and troublesome SC calculation. In this way, it is possible to solve two uncoupled Schrödinger-like equations. 3. Results 3.1. n-type DDD GaAs quantum wells The starting parameters for n-type DDD quantum wells are: m∗ =0.067, r =12.5, and 1×1012 ≤n2D ≤1×1013 cm−2 . In Fig. 1, the potential profile and the square of the wave functions are presented. The impurity density considered is n2D = 4 × 1012 cm−2 , first omitting the many-body effects (Fig. 1a), and after taking them into account (Fig. 1b). From Fig. 1a and 1b, it is possible to see the relative importance of the exchange effects, since when many-body effects are considered, the depth of the wells increases as well as the energy of electron levels does. In Fig. 2, the electron energy levels are sketched as function of the distance between wells, without (a), and with (b) exchange effects. The impurity concentration in this case is n2D = 1 × 1012 cm−2 . The main features of the energy levels are: • For l = 0 the energy level structure corresponds to a SDD quantum well. • As the impurity planes get apart, the electron energy levels go down energetically, i.e., the DDD quantum wells behave like a SDD quantum well, with the only F IGURE 1. Potential profile and electron eigenfunctions for n-type DDD GaAs quantum wells, (a) without and (b) with exchange effects (n2D = 4 × 1012 cm−2 ). Rev. Mex. Fı́s. 50 (6) (2004) 614–619 SUBBAND STRUCTURE COMPARISON BETWEEN N - AND P -TYPE DOUBLE DELTA-DOPED GAAS QUANTUM WELLS 617 In Table I the degeneracy distance (ldeg ), depth of the quantum wells (V0 ), and the degeneracy-energy difference between excited states and the ground level (E0 − E1 , E0 − E2 , etc) are given. We study three different impurity densities with (x) and without (o) exchange effects, in order to analyze the low, intermediate, and high density limits From Table I we can give a more general description: 1. Increasing the impurity density, the quantum well depth also augments. Thereby it is possible to bound more electron levels. 2. ldeg diminishes as the impurity density is increased. 3. The many-body effects are more important in the low density limit. 4. The exchange effects have also relevance in the estimation of the degeneracy-energy difference between the excited states and the ground level. F IGURE 2. Electron states versus the distance between the impurity planes l, for an impurity density of n2D = 1 × 1012 cm−2 , without (a) and with (b) many-body effects. F IGURE 3. SDD behavior of n-type DDD quantum wells, the impurity concentration considered is n2D = 1 × 1012 cm−2 (with exchange effects). • The energy levels go up, until the degeneration occurs and the level structure again corresponds to a SDD. In Ref. 25 a Si δ-layer with a concentration n2D =6.8 × 1012 cm−2 is studied experimentally by infrared excitation. The parity-allowed transitions have energies E1 − E0 =82.4 meV, and E3 − E0 = 126 meV. Our calculations (l=0) give for the same transitions values of 89 and 143 meV, respectively. The subband densities (ni ) measured are 4.7, 1.7, and 0.2 × 1012 cm−2 . Our results are n0 =4.3, n1 =1.7, and n2 =0.7 × 1012 cm−2 . Self-consistent one-electron calculations were performed [26], in which the input parameter was the experimental two-dimensional density of electrons in each level. By n2D =3 × 1012 cm−2 the difference between the levels are E1 − E0 =49 meV, E2 − E0 = 64.3 meV and E3 − E0 =71.5 meV. In our calculation (l= 0) E1 − E0 = 49.8, E2 − E0 = 67.1, and E3 − E0 =76.6 meV. The sub-band densities measured are 2.25, 0.5 and 0.1 × 1012 cm−2 . Our outputs (l = 0) are n0 = 1.2, n1 = 0.7, and n2 =0.2 × 1012 cm−2 . Magnetotransport measurements were made in Ref. 27, with n2D = 3 × 1012 cm−2 . The sub-band densities reported are 2.05 and 0.7 × 1012 cm−2 . Our results (l = 0) are 2.1 and 0.7 × 1012 cm−2 , respectively. A tunneling experiment was performed by Zachau and coworkers [28]. The basic level obtained is 181 meV (n2D =8 × 1012 cm−2 ). Our calculations give 186 meV (l=0). Kim et al. [29] measured subband densities, n0 =2.7 and n1 =0.7 (in units of 1012 cm−2 ) with n2D =(3.3 ± 4) × 1012 cm−2 . We obtain (l=0) n0 =2.5 and n1 =0.6. In all cases considered above our results are with exchange effects. 3.2. p-type DDD GaAs quantum wells In this case, the input parameters are: mhh = 0.52m0 , mlh = 0.087m0 , r = 12.5, and 1 × 1012 ≤ p2D ≤ 1 × 1013 cm−2 . In Fig. 4a and 4b the hole levels are given as function of the interlayer distance l. Rev. Mex. Fı́s. 50 (6) (2004) 614–619 618 I. RODRIGUEZ-VARGAS AND L.M. GAGGERO-SAGER TABLE II. The same as in Table I, but now for p-type DDD quantum wells, with ∆Ehh01 = Ehh0 − Ehh1 , ∆Ehl00 = Ehh0 − Elh0 , ∆Ehh02 = Ehh0 − Ehh2 , etc. p2D o ldeg Ehh0 Elh0 x ldeg Ehh1 Ehh0 Elh0 o ∆Ehh01 x ∆Ehh01 o ∆Ehl00 x ∆Ehl00 V0o V0x −8.1 −2.7 −4.6 −14.4 −21.9 Ehh1 1 340 230 4 150 440 400 130 350 340 −15.9 −22.6 −9.1 −12.6 −43.6 −58.8 10 90 300 260 90 270 220 −31.0 −40.8 −18.9 −34.8 −82.2 −105.9 F IGURE 4. Hole subband structure as a function of the interlayer distance between wells, omitting (a) and taking into account (b) exchange effects with p2D = 1 × 1012 cm−2 . By and large, the behavior of the hole levels in terms of l is the same as in the case of n-type DDD. However, two level ladders appear (hh and lh) and their degeneracy distances are very different as we can see from Figs. 4a and 4b. This depends directly on the effective masses, since the heavy hole mass is greater than the light hole mass, the degeneracy distance diminishes for hh levels as is shown in Figs. 4a and 4b. While for lh levels, the degeneracy distance resembles what happens when the carriers involved are electrons, because the effective mass of lh is approximately the same as for the electrons. Figures 5a and 5b sketch the potential profile and the F IGURE 5.Hole eigenfunctions and potential profile, for ptype DDD quantum wells considering exchange effects, for different interlayer distances: (a) 100 Å and (b) 280 Å, with p2D =4×1012 cm−2 . square of the wave functions for two distances between the impurity planes, (a) 100 Å and (b) 280 Å. The p-type DDD quantum wells is less deep than the ntype DDD. We can see this comparing Fig. 4a and 4b to Fig. 1b. Besides the hole energy levels are totally degenerated in Fig. 4b with respect to Fig. 4a. In Table II the main characteristics of p-type DDD are drafted. From this table, we have found that many-body effects are more important in p-type DDD with respect to the Rev. Mex. Fı́s. 50 (6) (2004) 614–619 SUBBAND STRUCTURE COMPARISON BETWEEN N - AND P -TYPE DOUBLE DELTA-DOPED GAAS QUANTUM WELLS n-type system (see Table I). In the low density limit, a difference of 90 Åbetween the degeneracy distance, with and without exchange effects is found, for the ground state of hh, while in n-type system this difference is 40 Å. Increasing the impurity density we can bound more hole levels, predominantly hh, because lh levels are more de-localized, i.e., the screening and localization is less effective for lh (as in the case of electrons) compared with hh. The p-type Alx Ga1−x As/GaAs/Alx Ga1−x As quantum wells were grown in Ref. 30, with p2D =8×10−2 cm−2 . They reported a subband separation of 36 meV. Although our calculations (l = 0) refers to a simpler system, we find an energy difference between first and second hh levels of 37 meV. Be δ-doped GaAs quantum wells were grown by Damen and coworkers [31], with p2D = 6 × 1012 cm−2 . The energy difference between the Fermi level and basic level is 22 meV. We obtain (l = 0) an energy difference of about 26 meV. PL spectroscopy study is performed in Ref. 32. Also SC calculations with p2D = 8 × 1012 cm−2 were performed. SC results are: Ehh0 − Elh0 = 15.1 meV. According to PL spectroscopy measurements this difference is 19 meV. Our calculation (l = 0) gives 20 meV. We obtain 14 meV with p2D = 3 × 1012 cm−2 , whereas the experimental result reported is 11 meV for the same impurity concentration. 1. C.E.C Wood, G. Metze, J. Berry, and L.F. Eastman, J. Appl. Phys. 51 (1980) 383. 2. K. Ploog, J. Cryst. Growth 81 (1987) 304. 3. E.F. Schubert, A. Fischer, and K. Ploog, IEEE Trans. Electron Devices 33 (1986) 625. 4. M. Zachau, F. Koch, K. Ploog, P. Roentegen, and H. Beneking, Solid State Commun. 59 (1986) 591. 5. K. Köhler, P. Ganser, and M. Maier, J. Cryst. Growth 127 (1993) 920. 6. L.M. Gaggero-Sager and R. Pérez-Alvarez, J. Appl. Phys. 74 (1995) 4566. 7. E.F. Schubert and K. Ploog, Jpn. J. Appl. Phys. 24 (1985) L608. 8. K. Nakagawa, A.A. van Gorkum, and Y. Shiraki, Appl. Phys. Lett. 57 (1989) 1869. 9. M. Hirai et al., J. Cryst. Growth 150 (1995) 209. 10. D.A. Woolf et al., J. Cryst. Growth 150 (1995) 197. 11. T. Iida et al., J. Cryst. Growth 150 (1995) 236. 12. L.M. Gaggero-Sager and R. Pérez-Alvarez, Phys. Stat. Sol. (b) 197 (1996) 105. 13. G.M. Siphai, P. Enderlein, L.M.R. Scolfaro, and J.R. Leite, Phys. Rev. B 53 (1996) 9930. 14. L.M. Gaggero-Sager and R. Pérez-Alvarez, J. Appl. Phys. 79 (1996) 3351. 15. N.Y. Li, H.K. Dong, C.W. Tu, and M. Geva, J. Cryst. Growth 150 (1995) 246. 16. L.M. Gaggero-Sager, Modelling and Simulation in Materials Science and Engineering 9 (2001) 1. 619 Gilinsky and colleagues [33] reported the PL spectrum in ptype Be δ-doped GaAs layers for 4 × 1012 , 1.8 × 1013 , and 3.6×1012 cm−2 , obtaining Ehh0 −Elh0 = 8, 20 and 30 meV, respectively. With the TFD theory (l = 0) we obtain 12.5, 35 and 55 meV. The discrepancy, as we can see from the high impurity concentrations, may be due to the impurity spreading. 4. Conclusions As a final comment, we can say that TF and TFD approximations are very useful tools in the study of semiconductor systems, such as n- and p-type DDD GaAs quantum wells. These theories permit us to obtain analytical expressions for the potential that represents the corresponding conduction and valence band bending. The electron and hole subband structure calculations reveal the main features of n- and ptype system. It is shown that exchange effects take more relevance in p-type DDD, since the screening is more effective, and the holes are more localized than in the case of electrons. Besides it is important to stress that the TFD theory is only applicable in p-type systems. Also our results agree with respect to the experimental data available. 17. L.M. Gaggero-Sager, Phys. Stat. Sol. (b) 231 (2002) 243. 18. S.J. Vlaev and L.M. Gaggero-Sager, Some Contemporary Problems of Condensed Matter Physics (Nova Science, 2000). 19. G.Q. Hai and N. Studart, Phys. Rev. B 52 (1995) 2245. 20. L.M. Gaggero-Sager, J.C. M’Peko, and R. Pérez-Alvarez, Rev. Mex. Fı́s. 47 (2001) 153. 21. E. Ozturk and I. Sokmen, J. Phys. D 36 (2003) 2457. 22. X. Zheng, T.K. Carns, K.L. Wang, and B. Wu, Appl. Phys. Lett. 62 504 (1993). 23. H.H. Radamson et al., Appl. Phys. Lett. 64 1842 (1994). 24. V.L. Gurtovoi, V.V. Valyaev, S. Yu. Shapoval, and A.N. Pustovit, Appl. Phys. Lett. 72 (1998) 1202. 25. C.A.C. Mendoca et al., Phys. Rev. B 48 (1993) 12316. 26. G. Tempel, F. Muller, N. Scharz, F. Koch, G. Weiman, H.P. Zeeindl, and I. Eisele, Surf. Sci. 228 (1990) 247. 27. J.C. Egues, A. Barbosa, A.C. Notari, P. Basmaji, L. Ioriatti, E. Ranz, and J. Portal, J. Appl. Phys. 70 (1991) 3678. 28. M. Zachau, F. Koch, K. Ploog, P. Roentgen, and H. Beneking, Solid State Commun. 59 (1986) 591. 29. T.W. Kim, K.-H. Yoo, K.-S. Lee, Y. Kim, S.-K. Min, S.S. Yom, and S.J. Lee, J. Appl. Phys. 76 (1994) 2863. 30. J. Wagner, A. Ruiz, and K. Ploog, Phys. Rev. B 43 (1991) 12134. 31. T.C. Damen et al., Appl. Phys. Lett. 67 (1995) 515. 32. D. Richards et al., Phys. Rev. B 47 (1993) 9629. 33. A.M. Gilinsky et al., Superlatt. Microstruct. 10 (1991) 399. Rev. Mex. Fı́s. 50 (6) (2004) 614–619